**Short Fatigue Crack Behavior of LZ50 Axle Steel under Rotating-Bending**

**Cyclic Loading**

**B. Yang,1S. Dai, Y. Y. Wu, Z. Liao, S. Liang, S. N. Xiao**

State Key Laboratory of Traction Power, Southwest Jiaotong University, Chengdu, China

1

yb@swjtu.cn

*The short fatigue short crack replica tests using LZ50 axle steel hourglass-shaped specimens of were*
*carried out under rotating-bending cyclic load. Seven sets of effective test data were obtained. The*
*analysis demonstrated that short fatigue cracks generally originate in ferrite grains or on their*
*boundaries, and then short cracks start propagating, which is strongly influenced by the microstructure*
*of the material. The crack growth rate increases serratically, followed by its decrease double-fold*
*because of the limit of ferrite grain boundaries and the banded pearlite structure. Based on the three*
*principles of the best fit, which include the overall fitting effect, correlation with fatigue physics, and*
*safety of residual strength prediction, the statistical evolution of the dominant effective short fatigue*
*crack length and life share were analyzed. The statistical results show that the minimum value*
*distribution exhibit the best fit of the dominant effective fatigue short crack length and the life share.*
*The short fatigue crack growth model, which includes various microstructure barriers, provides a*
*good fitting result and reflects the cyclic effect of the microstructure on the short fatigue crack*
*behavior.*

* Keywords*: fatigue, short crack, rotating-bending load, LZ50 axle steel.

**Introduction.** Fatigue and fracture are the main causes of the failure of engineering
structures and components [1]. The prediction of the behavior of fatigue cracks by the
linear elastic fracture mechanics (LEFM) is limited, since it fails to describe the observed
propagation patterns of short fatigue cracks [2]. Numerous experimental results show that
for components with a smooth surface, the initiation and growth of short fatigue cracks
occupy over 80% of their total fatigue life [3]. Therefore, it is of great importance to study
the initiation and growth of short fatigue cracks, which has important engineering
significance for the accurate prediction the component fatigue life values.

The axle is the key bearing component of locomotives and vehicles, which is subjected to a number of complex stresses, such as rotating-bending and impact during running so that the fatigue cracking is the main form of failure. With the improvement of science and technology, the passenger and freight volume of railway vehicles is increasing as well as the running speed. Consequently, the alternating loads of axles are becoming more and more complicated and seriously influence the traffic safety. In present study, the behavior of short fatigue crack for LZ50 axle steel under rotating-bending load is studied. Based on the replica tests and observation data from laser scanning confocal microscope, there is a good understanding for the behavior of short fatigue crack. The specific work is as follows:

(i) the short fatigue crack replica tests under rotating-bending load have carried out and the process of short fatigue crack initiation and growth under rotating-bending load have been revealed by the analysis of the experimental results;

(ii) the statistical evolution of the dominant effective fatigue short crack (DESFC) scale and life share for LZ50 axle steel under rotating-bending load has been analyzed;

(iii) based on the short fatigue crack growth model which includes various micro-structure barriers, the short crack growth rate under rotating-bending load is fitted and compared with the experimental data.

**1. Experimental Details.**

* 1.1. Materials and Specimens.*The specimens are made from LZ50 axle steel which
is originated from a RE2B type axle. The originally cylindrical specimens were processed
to obtain the hourglass shape, as shown in Fig. 1. The minimum diameter of the specimen
was 6 mm and the intermediate part was polished to reduce the surface roughness. The
heat-treatment conditions were as follows: normalizing heating for 2 h under 860 and
800°C, tempering for 1.5 h under 570°C according to the Chinese standard [4]. The
chemical composition (wt.%) of LZ50 axle steel was 0.47 C, 0.78 Mn, 0.26 Si, 0.15 Cu,
0.028 Ni, 0.021 Al, 0.02 Cr,<0.014 P, and<0.007 S. The mechanical properties at room
temperature were as follows: 209.750 GPa for elastic modulus, 628.96 MPa for tensile
strength, 329.94 MPa for yield strength, 24.41% for elongation, 41.92% for reduction of
area, and 44 J/cm2 for impact toughness.

* 1.2. Metallographic Tests.* The metallographic tests of LZ50 steel specimens were
conducted, which showed its composition, including ferrite and lamellar pearlite (Fig.
2b). Due to forging used in the process of material smelting, the pearlite had a banded
structure (Fig. 2a). The measured equivalent diameters of ferrite and pearlite were
13.12 and 14.83 mm, while the average spacing of the banded pearlite structure was
64.59 mm.

* 1.3. Replica Tests.* All replica tests were performed using a PQ-6 rotating bending
fatigue machine under sine loading wave with the loading frequency of 50 Hz. The
maximum nominal stress was controlled to be 310 MPa and the stress ratio was equal to

*R*=-1 [5]. Each test involved one specimen, which was evenly engraved with a depth of

Fig. 1. Schematic of shape and dimension of the specimen (unit: mm).

a b

about 5 mm by longitudinal scratches in the middle of the smooth part. These scratches
were used as marks, which would not affect the specimen life, but were instrumental in the
short crack detection and location by the microscopic observation [6–9]. Installing the
specimen on the machine and then turning on the power, the replica test started. In the
process of loading, the test would be interrupted at a predetermined cycle number. Then,
cellulose acetate film softened with methyl acetate was pasted on the specimen middle
surface. Once the methyl acetate was completely evaporated, the film, which reflected the
appearance morphology of the specimen surface, was carefully removed with tweezers.
Finally, the dried film was placed between two glass plates. The predetermined cycle
numbers of tests were as follows: 0–0.2*w*–0.5*w*–1*w*–3*w*–5*w*–10*w*-15*w*–20*w*–25*w*–30*w*–
35*w*–40*w*–fracture (where*w* represents 104 cycles).

Eventually, seven effective specimens were obtained and their replicas were examined step-by-step, according to the reverse observation method using Olympus OSL4100 laser scanning confocal microscope, to investigate the behavior of short fatigue cracks under rotating-bending cyclic load. The fatigue fracture surface features (striations) were observed using the scanning electron microscope (SEM).

**2. Description of Short Crack Behavior.**

* 2.1. Observation of Typical Specimen.*Take the typical specimen B-2 as an example,
the fatigue life of B-2 is 363,726 cycles and there are a total of 12 replica films. Figure 3
shows the growth of short cracks for B-2 specimen. Based on the “effective short fatigue
criterion” proposed by Zhao [10, 11], the behavior of short fatigue crack under
rotating-bending cyclic load is described below (

*C*is effective short fatigue crack and

*F*is ineffective short fatigue crack):

(a)*N*=0 cycles, at which point the specimen bears no load, so there are few surface
defects, except for some vertical lines, which are very shallow and parallel with each other.
This is because the polishing process will produce a pattern in the specimen surface by
pressure and form the reflection of these lines like traces.

(b) *N*=30,013 cycles, short fatigue cracks *C1*, *C2*, and *F1* were nucleated in the
ferrite grain. The lengths of*C1*and*C2*are about 20 mm, while the length of*F1*is slightly
smaller ( of about 7 mm). As compared with the equivalent diameters of ferrite (between
4.41 and 27.61 mm, and the average is 13.12 mm) measured previously, it is found that
lengths of these three short cracks are equivalent to the equivalent diameters of ferrite.

(c)*N*=150,012 cycles, the crack tip of*C1*breaks through the ferrite grain boundary
and begins to grow at both ends, reaching a length of 57.970mm, while*C2*and*F1*are still
limited within the ferrite grain and controlled by their respective grain.

(d) *N*=200,013 cycles,*C1*begins to grow quickly to a length of 101.922 mm which
is close to the spacing of pearlite banded structure (between 47.58 and 129.66 mm, and the
average is 64.5 mm) while*C2*and*F1*are not extended and cannot get rid of the limit of
ferrite grain because lack of energy.

(e) *N*=250,008 cycles, *C1* continues to grow strongly to a length of 171.117 mm.
And now*C2*has got rid of the limit of ferrite grain with the crack tips break through the
boundary. The length of*C2*has reached to 89.775mm. There is a phenomenon that should
be noticed that *C1* and *C2* have a tendency to merge which will be combined to the
DESFC. *F1* does not grow either.

(f) *N*=300,014 cycles, *C1*and *C2*have combined to a new crack, the DESFC*C1*,
and its length now is 647.887 mm. And the crack*F1*which grew slowly before has a large
growth to the length of 83.281 mm. Perhaps the limit of ferrite grain boundary has been
broken. Below the left of *C1*’s crack tip, there is a new crack *F2*.

(g) *N*=350,040 cycles,*C1* has formed to the traditional long crack, and with the
accumulation of damage,*C1*continues to grow, but its growth path is not a straight line
because the inclusions and other obstacles may influence the growth process. In general,
the growth of*C1*is along the direction perpendicular to the stress. Although the crack tips

are still limited by the ferrite grain boundary or grain, their limiting effect is insufficient to
limit the growth of the dominant effective short fatigue crack. And two new cracks*F3*and
*F4* can be seen in the field of view. Besides, the growths of *F1* and *F2* are greatly
suppressed by the predominance of DESFC so that both of them stop growing.

a b c d e f g

Fig. 3. OM images of replica films of fatigue short crack initiation and propagation for typical specimen under rotating-bending cyclic load.

* 2.2. Observation of Fatigue Fracture.* Figure 4 shows some scanning electron
microscope (SEM) images of different areas of the fatigue fracture for typical specimen
B-2 with different magnification. As displayed, Fig. 4a shows the full view of the fracture
and the crack initiation lies in the bottom left corner of the view which begins from the
specimen surface while the fatigue final rupture region is located opposite with a deflection
angle. Figure 4b shows the fatigue source zone and crack growth zone at low magnification
and fatigue striations appearance sourced from crack initiation can be observed. These
striations represent the propagation of the short crack. Figure 4c shows the secondary
cracks in crack growth zone at high magnification which are approximately perpendicular
to the direction of the crack growth path. And many tear dimples can be seen obviously in
transient breaking zone in Fig. 4d.

* 2.3. Analysis of Typical Specimens.*The relationship between the DESFC length and
its fatigue life share of three typical specimens B-2, B-4, and B-5 is depicted in Fig. 5,
while Figs. 6 and 7 show the variation of DESFC growth rate with the crack length and
fatigue life share under rotating-bending load. Taking specimen B-2 as an example, and
combining with images of replica films (Fig. 3) and SEM images of fatigue fracture (Fig. 4),
the following conclusions can be drawn:

In the whole fatigue life of the specimen, the length of DESFC increases with the number of load cycles without any stagnation (Fig. 5). During the first half the fatigue life, DESFC grows quite slowly, resulting in that the change of DESFC length in the first 50% life is just 2.1% of the change of DESFC length in the last 50% life. In other words, most of the fatigue life is consumed in the crack initiation phase. During the whole process, the

a b

c d

crack growth rate increases with fluctuations, but it clearly exhibits two decelerations. As seen from Figs. 6 and 7, the data indicate that when the first deceleration of the growth rate happens, its corresponding life share is 0.014 and the corresponding projection length of DESFC is 14.149 mm, which is close to the equivalent diameter of the ferrite grain. The ferrite grain boundary acts as a barrier because the adjoining pearlite has much higher microhardness. This phenomenon occurs in the stage b ~ c in Fig. 3. When the second deceleration of the growth rate happens, its corresponding life share is 0.411 and the corresponding projection length of DESFC is 75.133 mm, which is close to the average spacing of pearlite banded structure. Also because of the higher hardness, the layered pearlite banded structure appears another barrier for the crack to overcome. This phenomenon occurs at stage d ~ e in Fig. 3. With these analyses, the conclusion can be drawn that the growth of short fatigue crack will influence by the ferrite boundary and the pearlite banded structure and when breaking these barriers, the growth rate of short fatigue crack will decrease and then rise again when breaking through the barriers.

Generally speaking, the overall trend of the curves showed in Figs. 5–7 for these three specimens is consistent, but due to the inherent difference of individual characteristic microstructural sizes, these curves do not overlap with each other completely. When the deceleration occurs, the corresponding DESFC length and life share are somewhat dispersed.

Fig. 5 Fig. 6

Fig. 5. Variation curve of DESFC scales with life share for typical specimens.

Fig. 6. Variation curve of DESFC growth rate with DESFC length for typical specimens.

**3. Statistical Analysis.**In order to determine the reasonable assumed discriminations
and the statistical evolution of short fatigue crack behavior for LZ50 axle steel under
rotating-bending cyclic load, authors [12] proposed a unified linear regression method,
which includes the following three aspects: (i) the total fitting effect which measured with a
uniform parameter by quantitative analysis and the best will be selected; (ii) the consistency
with the relevant fatigue physics (e.g., when fitting the crack length, the longer the crack,
the higher the probability of failure); (iii) the safety of design evaluation. The two
characteristic parameters, statistical evolution of DESFC length and life share, have been
analyzed in this study by comparing six commonly used distributions, including
three-parameter Weibull distribution (3PWD), two-parameter Weibull distribution (2PWD),
normal distribution (ND), lognormal distribution (LND), extreme minimum distribution
(EMVD1), and extreme maximum distribution (EMVD2).

* 3.1. The Statistics Evolution of DESFC Length.* The mean value (

*Am*), standard

deviation (*As*), and variation coefficient (*VA*) of DESFC length are given in Table 1. As for

the total fitting effect, the closer the absolute value of linear correlation coefficient, namely
*RXY* , gets to one, the better the fitting effect is [12]. By comparison, it is found that among

the 10 groups of DESFC length data listed in Table 1, EMVD1 has the best fitting effect for
6 groups. Then considering the safety of design evaluation, reference [12] defines two
parameters, *dF*1 and *dF*2, to reflect the prediction deviation. For EMVD1, 5 groups of
data show that *dF*1<*dF*2 and 9 groups of data show that *dF*1<1, which means that the
predicted values will be relatively conservative and safe. At the same time, the EMVD1
conforms to the correlation with the relevant fatigue physics, i.e., with the increase of the
growth rate, the failure probability will also increase. In conclusion, EMVD1 shows a
better consistency with the criteria described in study [12] than other five distributions, and
therefore is a good fit of the DESFC length. Corresponding cumulative distribution curve is
shown in Fig. 8a. With the increase of the life share, the length of DESFC increases and the
curve of variation coefficient are sine-shaped which fluctuates up and down at 0.3 and
reaches the minimum when the life share is 0.9. So there is a large scatter of the DESFC
length and the growth of DESFC is not stable at all stages.

T a b l e 1

**Basic Statistical Parameters of DESFC Length under Rotating-Bending Load**

*f* *A _{m}*, mm

*A*, mm

_{s}*V*0.1 20.431 5.918 0.290 0.2 28.006 9.066 0.324 0.3 36.122 13.396 0.371 0.4 58.164 18.573 0.319 0.5 99.703 40.265 0.404 0.6 185.570 74.144 0.400 0.7 328.607 91.306 0.278 0.8 814.433 294.689 0.362 0.9 1797.381 273.352 0.152 1.0 2986.122 636.993 0.213

_{A}* 3.2. The Statistics Evolution of Fatigue life share.* The mean value (

*fm*), standard

deviation (*f _{s}*), and variation coefficient (

*V*) of fatigue life share are given in Table 2. The statistics evolution of fatigue life share is analyzed using the same approach as described above. It is found that among the 12 groups of life share data, EMVD1 has the best fitting effect for 5 groups of data, while 11 groups of data show that

_{f}*d*

_{F}_{1}<

*d*

_{F}_{2}. Besides, just as mentioned in Subsection 3.1, EMVD1 conforms to the consistency with the relevant fatigue physics. It can be concluded that EMVD1 is a good assumed distribution of fatigue life share. Corresponding cumulative distribution curve is shown in Fig. 8b. With the increase of DESFC length, the fatigue life share increases, while the variation coefficient decreases constantly from 0.635, then stabilize for a certain period of time, and eventually tend to zero. So, initially, a large dispersion of the fatigue life share is observed, which gradually exhibit a saturation and approach zero.

T a b l e 2

**Basic Statistical Parameters of Fatigue Life under Rotating-Bending Load**

2*a*, mm *f _{m}*

*f*

_{s}*V*20 0.1080 0.0686 0.6354 50 0.3746 0.0749 0.1999 100 0.5091 0.0725 0.1424 150 0.5747 0.0570 0.0992 300 0.6789 0.0520 0.0766 500 0.7536 0.0251 0.0333 700 0.7917 0.0397 0.0501 800 0.8023 0.0372 0.0464 900 0.8127 0.0349 0.0429 1000 0.8230 0.0337 0.0409 1500 0.8692 0.0273 0.0314 2000 0.9041 0.0175 0.0194 a b

_{f}Fig. 8. Extreme minimum value distribution probability curves of DESFC length (a) and fatigue life share (b).

**4. Short Crack Growth Model.**To refine the short fatigue crack growth concept and
analyze it quantitatively, it is necessary to establish the short crack growth model. Based on
the foregoing study, it can be confirmed that the behavior of short fatigue crack for LZ50
axle steel under rotating-bending cyclic load is mainly controlled by the material
microstructure. Given this, the short fatigue crack growth model of Yang et al. [13, 14],
which accounts for various microstructure barriers, was selected as follows:

*da*
*dN* *G* *A* *W at* *Wt* *fi* *di* *di*
*i*
*n* *m*
= + é
-ë
ê
ê
ù
û
ú
ú
=

### å

0 1 D D (D ) , (1)where *a* is DSSEC length, *N* number of cycles, *G*0 is the basic growth rate in each
microstructure and, in general, it is the minimum value of growth rate in the first
microstructural barrier period, D*Wt* is the far field total cyclic strain energy density, *di* is

the length of characteristic microstructural barrier, *i* is the subscript to clarify the kinds of
barriers, *A* and *m* are constants relating to materials, and *f*(D*di*) is the resistance

coefficient function.

The microstructure barriers of LZ50 axle steel in this study are reduced to only two
types, which are the ferrite grain boundary and the pearlite banded structure. When
conducting the replica tests, the nominal stress on the surface of the specimen is controlled,
so the far field total cyclic strain energy density D*Wt* can be expressed by constant in the

respective equation. Given this, the simplified models take the following forms:
*da*
*dN* *G* *A a* *f* *d* *d*
*m*
= 01+ 1[ - 1(D 1) 1] 1, (2)
*da*
*aN* *G* *A a* *f* *d* *d*
*m*
= 02+ 2[ - 2(D 2) 2] 2, (3)

where *d*1 is the equivalent diameter of ferrite grains and *d*2 is average spacing of banded
pearlite structures.

Based on the seven sets of effective test data obtained from the replica tests, all required characteristic parameters of the growth model were obtained and listed in Table 3. The respective fitting curve is depicted in Fig. 9 and is coincident with most of the test data points, which means the overall fitting effect is good and the two evident decelerations are exhibited correctly. Furthermore, the statistical processing of the test data yields that the short crack growth rate at the early stage has a large scatter because of strong microstructure effect, which scatter diminishes at the later stage, when a long crack is formed.

T a b l e 3

**Parameters of Short Fatigue Crack Growth Model Considering All Valid Specimens**

Parameter *d*_{1}, mm *G*_{01}, m/cycle *A*_{1} *m*_{1} a_{1}

Value 23.64 7 08 10. × -11 6 33 10. × -9 2.52 0.55

Parameter *d*_{2}, mm *G*_{02}, m/cycle *A*_{2} *m*_{2} a_{2}

**C o n c l u s i o n s**

1. Under the rotating-bending cyclic load, short fatigue cracks in LZ50 axle steel mainly originate in the ferrite grain boundary or within the ferrite grains, and their growth is strongly influenced by the material microstructure. The overall growth rate of short fatigue crack increases, but there are two typical decelerations because of the limit of the ferrite grain boundary and the banded pearlite structure. As soon as the short fatigue crack breaks the barrier of the banded pearlite structure, its growth behavior coincides with that of long cracks and complies with LEFM.

2. The initiation of short fatigue cracks takes the major part of the total fatigue life because the DESFC length augmentation in the first half of life is about 2.1% of that in the second half.

3. Both characteristic parameters (DESFC length and fatigue life share) grow in the loading process and have large scatters, which are best-fitted via EMVD1 distribution.

4. Based on the short fatigue crack growth model, which accounts for multiple microstructure barriers, the calculated were effectively fitted with the test data.

* Acknowledgments.* Present work is supported by the National Key R&D Program of
China (2016YFB1200403), the National Natural Science Foundation of China (51675446
and U1534209), and the Opening Project of State Key Laboratory of Traction Power (grant
No. 2015TPL_T13).

1. C. Y. Chen,*Fatigue and Fracture*[in Chinese], Huazhong University of Science and
Technology Press, Hubei (2001).

2. S. Suresh, *Fatigue of Materials*, Cambridge University Press (1998).

3. Y. S. Hong and B. Fang, “The mesoscopic process and theory of short fatigue cracks
initiation and propagation,” *Adv. Mech.*,**23**, 468–486 (1993).

4. *TB/T 2945-1999. LZ50 Axle Railway Vehicle and Steel Billets Technical Conditions*,
Chinese Standard, Implemented on September 1, 1999.

5. B. Q. Ma, *Comparison of Short Fatigue Crack Behavior for LZ50 Axle Steel under*
*Two Different Loading Frequencies* [in Chinese], Southwest Jiaotong University,
Chengdu (2016).

Fig. 9. Fitting curve of short fatigue growth model for all valid specimens under rotating-bending cyclic load.

6. Y. X. Zhao, Q. Gao, and J. N. Wang, “Experimental observation on the short fatigue
crack behavior of a stainless steel pipe-weld metal I – Material microstructures and
research approach,” *Acta Metall. Sin.*, **36**, 931–936 (2000).

7. Y. X. Zhao, Q. Gao, J. N. Wang, “Experimental observation on the short fatigue crack
behavior of a stainless steel pipe-weld metal II – Crack initiation, growth and
interaction,”*Acta Metall. Sin*., **36**, 937–943 (2000).

8. Y. X. Zhao, B. Yang, and Q. Gao, “Initiation and early propagation of short fatigue
cracks on weld metal of 1Cr18Ni9Ti pipes,”*Nucl. Power Eng.*,**24**, 127–132 (2003).
9. Y. X. Zhao, B. Yang, and Q. Gao, “Experiment of physical short fatigue crack

propagation of 1Cr18Ni9Ti weld metal,” *Nucl. Power Eng.*, **26**, 584–589 (2005).
10. Y. X. Zhao, *Analysis of Low Cycle Fatigue Short Crack Behavior and Reliability*,

PhD Thesis, Southwest Jiaotong University, Chengdu (1998).

11. Y. X. Zhao, B. Yang, and Q. Gao. “Equation of short fatigue crack growth law of
1Cr18Ni9Ti weld metal,”*Nucl. Power Eng.*,**26**, 590–597 (2005).

12. Y. X. Zhao, Y. F. Sun, and Q. Gao, “Unified linear regression method for the analysis
of seven commonly used statistical distribution,” *J. Mech. Strength.*, **23**, 102–106
(2001).

13. B. Yang and Y. X. Zhao, “Experimental research on dominant effective short fatigue
crack behavior for railway LZ50 axle steel,”*Int. J. Fatigue*, **35**, 71–78 (2016).
14. B. Yang, B. Q. Ma, S. N. Xiao, and Y. X. Zhao, “A probabilistic model for describing

short fatigue crack growth behavior of LZ50 steel,”*Strength Mater.*,**48**, No. 1, 90–97
(2016).

Received 15. 09. 2017